LMucko/crystallography-open-database huggingface dataset:
High internal stresses in Sr1-x La1+x Al1-x Mgx O4 solid solution (0 <= x <= 0.7) characterized by infrared and Raman spectroscopies coupled with crystal structure refinement
Magrez, A.; Cochet, M.; Ganne, M.; Joubert, O.; Louarn, G.; Chauvet, O.; Chemistry of Materials (1,1989-) 13 (2001) 3893–3898; doi:

data_4002322
_publ_section_title
;
 High internal stresses in Sr1-x La1+x Al1-x Mgx O4 solid solution (0 <= x
 <= 0.7) characterized by infrared and Raman spectroscopies coupled with
 crystal structure refinement
;
_journal_name_full               'Chemistry of Materials (1,1989-)'
_journal_page_first              3893
_journal_page_last               3898
_journal_volume                  13
_journal_year                    2001
_chemical_formula_sum            'Al0.3 La1.7 Mg0.7 O4 Sr0.3'
_chemical_name_systematic        '(Sr0.3 La1.7) (Al0.3 Mg0.7) O4'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.84414
_cell_length_b                   3.84414
_cell_length_c                   12.671
_cell_volume                     187.245
_citation_journal_id_ASTM        CMATEX
_cod_data_source_file            Magrez_CMATEX_2001_1456.cif
_cod_data_source_block           Al0.3La1.7Mg0.7O4Sr0.3
_cod_original_cell_volume        187.2446
_cod_database_code               4002322
X-ray powder diffraction data and Rietveld refinement for Ln6 W O12(Ln = Y, Ho)
Diot, N.; Benard-Rocherulle, P.; Marchand, R.; Powder Diffraction 15 (2000) 220–226; doi:

data_1525900
_publ_section_title
;
 X-ray powder diffraction data and Rietveld refinement for Ln6 W O12(Ln =
 Y, Ho)
;
_journal_name_full               'Powder Diffraction'
_journal_page_first              220
_journal_page_last               226
_journal_volume                  15
_journal_year                    2000
_chemical_formula_sum            'O12 W Y6'
_chemical_name_systematic        'Y6 O6 (W O6)'
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   9.7505
_cell_length_b                   9.7505
_cell_length_c                   9.3094
_cell_volume                     766.489
_citation_journal_id_ASTM        PODIE2
_cod_data_source_file            Diot_PODIE2_2000_454.cif
_cod_data_source_block           O12W1Y6
_cod_original_cell_volume        766.4892
_cod_original_formula_sum        'O12 W1 Y6'
_cod_database_code               1525900
The crystal structure of Cu2.31 Te S0.32 - a condensed cluster compound
Makovicky, E.; Karup-Moller, S.; Sotofte, I.; Zeitschrift fuer Kristallographie (149,1979-) 215 (2000) 475–480; doi:

data_8103609
_publ_section_title
;
 The crystal structure of Cu2.31 Te S0.32 - a condensed cluster compound
;
_journal_name_full
'Zeitschrift fuer Kristallographie (149,1979-)'
_journal_page_first              475
_journal_page_last               480
_journal_volume                  215
_journal_year                    2000
_chemical_formula_sum            'Cu2.307 S0.314 Te'
_chemical_name_systematic        'Cu2.307 Te S0.314'
_space_group_IT_number           210
_symmetry_space_group_name_Hall  'F 4d 2 3'
_symmetry_space_group_name_H-M   'F 41 3 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            48
_cell_length_a                   14.836
_cell_length_b                   14.836
_cell_length_c                   14.836
_cell_volume                     3265.506
_citation_journal_id_ASTM        ZEKRDZ
_cod_data_source_file            Makovicky_ZEKRDZ_2000_818.cif
_cod_data_source_block           Cu2.307S0.314Te1
_cod_original_formula_sum        'Cu2.307 S0.314 Te1'
_cod_database_code               8103609
X-ray powder diffraction data and Rietveld refinement for Ln6 W O12(Ln = Y, Ho)
Diot, N.; Benard-Rocherulle, P.; Marchand, R.; Powder Diffraction 15 (2000) 220–226; doi:

data_1525901
_publ_section_title
;
 X-ray powder diffraction data and Rietveld refinement for Ln6 W O12(Ln =
 Y, Ho)
;
_journal_name_full               'Powder Diffraction'
_journal_page_first              220
_journal_page_last               226
_journal_volume                  15
_journal_year                    2000
_chemical_formula_sum            'Ho6 O12 W'
_chemical_name_systematic        'Ho6 O6 (W O6)'
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   9.7583
_cell_length_b                   9.7583
_cell_length_c                   9.3142
_cell_volume                     768.112
_citation_journal_id_ASTM        PODIE2
_cod_data_source_file            Diot_PODIE2_2000_455.cif
_cod_data_source_block           Ho6O12W1
_cod_original_cell_volume        768.1119
_cod_original_formula_sum        'Ho6 O12 W1'
_cod_database_code               1525901
Structural properties of ferromagnesian cordierites
Malcherek, T.; McCammon, C.; Tazzoli, V.; Ottolini, L.; Domeneghetti, M.C.; Carpenter, M.A.; American Mineralogist 86 (2001) 66–79; doi:

data_1525902
_publ_section_title
;
 Structural properties of ferromagnesian cordierites
;
_journal_name_full               'American Mineralogist'
_journal_page_first              66
_journal_page_last               79
_journal_volume                  86
_journal_year                    2001
_chemical_formula_sum
'C0.165 H0.24 Al3.992 Fe0.55 Mg1.464 Na0.05 O18.45 Si4.994'
_chemical_name_systematic
;
(Mg0.732 Fe0.268)2 Na0.05 (Al3.992 Fe0.014 Si4.994) O18  (H2 O)0.12 (C O2)0.165
;
_space_group_IT_number           66
_symmetry_space_group_name_Hall  '-C 2 2c'
_symmetry_space_group_name_H-M   'C c c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   17.109
_cell_length_b                   9.7423
_cell_length_c                   9.3318
_cell_volume                     1555.434
_citation_journal_id_ASTM        AMMIAY
_cod_data_source_file            Malcherek_AMMIAY_2001_892.cif
_cod_data_source_block
C0.165H0.24Al3.992Fe0.55Mg1.464Na0.05O18.45Si4.994
_cod_original_formula_sum
;
C0.165 H0.24 Al3.992 Fe0.55 Mg1.464 Na0.05 O18.45 Si4.994
;
_cod_database_code               1525902
In situ Untersuchungen der Reaktion von Ammoniummonomolybdat, (N H4)2 Mo O4, mit Ammoniak: die Struktur von (N H4)2 (Mo3 O10)
Dittmann, M.; Schweda, E.; Zeitschrift fuer Anorganische und Allgemeine Chemie 626 (2000) 569–573; doi:

data_1525903
_publ_section_title
;
 In situ Untersuchungen der Reaktion von Ammoniummonomolybdat, (N H4)2 Mo
 O4, mit Ammoniak: die Struktur von (N H4)2 (Mo3 O10)
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              569
_journal_page_last               573
_journal_volume                  626
_journal_year                    2000
_chemical_formula_sum            'H8 Mo3 N2 O10'
_chemical_name_systematic        '(N H4)2 (Mo3 O10)'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 98.833
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   13.982
_cell_length_b                   8.041
_cell_length_c                   9.21
_cell_volume                     1023.193
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Dittmann_ZAACAB_2000_791.cif
_cod_data_source_block           H8Mo3N2O10
_cod_database_code               1525903
Structural properties of ferromagnesian cordierites
Malcherek, T.; Tazzoli, V.; Domeneghetti, M.C.; Ottolini, L.; Carpenter, M.A.; McCammon, C.; American Mineralogist 86 (2001) 66–79; doi:

data_1525904
_publ_section_title
;
 Structural properties of ferromagnesian cordierites
;
_journal_name_full               'American Mineralogist'
_journal_page_first              66
_journal_page_last               79
_journal_volume                  86
_journal_year                    2001
_chemical_formula_sum
'Al3.982 Fe1.265 H0.96 Li0.04 Mg0.716 Na0.091 O18.48 Si4.989'
_chemical_name_systematic
;
(Mg0.358 Fe0.618 Li0.02)2 Na0.091 (Al3.982 Fe0.029 Si4.989) O18 (H2 O)0.48
;
_space_group_IT_number           66
_symmetry_space_group_name_Hall  '-C 2 2c'
_symmetry_space_group_name_H-M   'C c c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   17.1735
_cell_length_b                   9.7859
_cell_length_c                   9.3113
_cell_volume                     1564.840
_citation_journal_id_ASTM        AMMIAY
_cod_data_source_file            Malcherek_AMMIAY_2001_893.cif
_cod_data_source_block
H0.96Al3.982Fe1.265Li0.04Mg0.716Na0.091O18.48Si4.989
_cod_original_cell_volume        1564.84
_cod_original_formula_sum
;
H0.96 Al3.982 Fe1.265 Li0.04 Mg0.716 Na0.091 O18.48 Si4.989
;
_cod_database_code               1525904
Structure of Pb (Zr, Ti) O3 near the morphotropic phase boundary
Dmowski, W.; Egami, T.; Davies, P.K.; Farber, L.; AIP Conference Proceedings 582 (2001) 33–44; doi:

data_1525905
_publ_section_title
;
 Structure of Pb (Zr, Ti) O3 near the morphotropic phase boundary
;
_journal_name_full               'AIP Conference Proceedings'
_journal_page_first              33
_journal_page_last               44
_journal_volume                  582
_journal_year                    2001
_chemical_formula_sum            'O3 Pb Ti'
_chemical_name_systematic        'Pb (Ti O3)'
_space_group_IT_number           99
_symmetry_space_group_name_Hall  'P 4 -2'
_symmetry_space_group_name_H-M   'P 4 m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.90044
_cell_length_b                   3.90044
_cell_length_c                   4.15115
_cell_volume                     63.153
_citation_journal_id_ASTM        APCPCS
_cod_data_source_file            Dmowski_APCPCS_2001_1445.cif
_cod_data_source_block           O3Pb1Ti1
_cod_original_cell_volume        63.15324
_cod_original_formula_sum        'O3 Pb1 Ti1'
_cod_database_code               1525905
The refinement of the crystal structure of skutterudite, Co As3
Mandel, N.; Donohue, J.; Acta Crystallographica B (24,1968-38,1982) 27 (1971) 2288–2289; doi:

data_2106188
_publ_section_title
;
 The refinement of the crystal structure of skutterudite, Co As3
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              2288
_journal_page_last               2289
_journal_volume                  27
_journal_year                    1971
_chemical_formula_sum            'As3 Co'
_chemical_name_systematic        'Co As3'
_space_group_IT_number           204
_symmetry_space_group_name_Hall  '-I 2 2 3'
_symmetry_space_group_name_H-M   'I m -3'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.195
_cell_length_b                   8.195
_cell_length_c                   8.195
_cell_volume                     550.360
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            Mandel_ACBCAR_1971_375.cif
_cod_data_source_block           As3Co1
_cod_original_cell_volume        550.3599
_cod_original_formula_sum        'As3 Co1'
_cod_database_code               2106188
Structure of Pb (Zr, Ti) O3 near the morphotropic phase boundary
Dmowski, W.; Egami, T.; Farber, L.; Davies, P.K.; AIP Conference Proceedings 582 (2001) 33–44; doi:

data_1525906
_publ_section_title
;
 Structure of Pb (Zr, Ti) O3 near the morphotropic phase boundary
;
_journal_name_full               'AIP Conference Proceedings'
_journal_page_first              33
_journal_page_last               44
_journal_volume                  582
_journal_year                    2001
_chemical_formula_sum            'O3 Pb Ti0.6 Zr0.4'
_chemical_name_systematic        'Pb (Zr0.4 Ti0.6) O3'
_space_group_IT_number           99
_symmetry_space_group_name_Hall  'P 4 -2'
_symmetry_space_group_name_H-M   'P 4 m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.992
_cell_length_b                   3.992
_cell_length_c                   4.1758
_cell_volume                     66.546
_citation_journal_id_ASTM        APCPCS
_cod_data_source_file            Dmowski_APCPCS_2001_1446.cif
_cod_data_source_block           O3Pb1Ti0.6Zr0.4
_cod_original_cell_volume        66.54581
_cod_original_formula_sum        'O3 Pb1 Ti0.6 Zr0.4'
_cod_database_code               1525906
Neutron and synchrotron diffraction study of U Pt Ge
Mannix, D.; Kawamata, S.; Coad, S.; Lander, G.H.; Brown, P.J.; Paixao, J.A.; Yamaguchi, Y.; Rebizant, J.; Langridge, S.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 62 (2000) 3801–3809; doi:

data_1525907
_publ_section_title
;
 Neutron and synchrotron diffraction study of U Pt Ge
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              3801
_journal_page_last               3809
_journal_volume                  62
_journal_year                    2000
_chemical_formula_sum            'Ge Pt U'
_chemical_name_systematic        'U Pt Ge'
_space_group_IT_number           44
_symmetry_space_group_name_Hall  'I 2 -2'
_symmetry_space_group_name_H-M   'I m m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.32
_cell_length_b                   7.17
_cell_length_c                   7.5
_cell_volume                     232.308
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            Mannix_PRBMDO_2000_481.cif
_cod_data_source_block           Ge1Pt1U1
_cod_original_formula_sum        'Ge1 Pt1 U1'
_cod_database_code               1525907
Structure of Pb (Zr, Ti) O3 near the morphotropic phase boundary
Dmowski, W.; Egami, T.; Davies, P.K.; Farber, L.; AIP Conference Proceedings 582 (2001) 33–44; doi:

data_1525908
_publ_section_title
;
 Structure of Pb (Zr, Ti) O3 near the morphotropic phase boundary
;
_journal_name_full               'AIP Conference Proceedings'
_journal_page_first              33
_journal_page_last               44
_journal_volume                  582
_journal_year                    2001
_chemical_formula_sum            'O3 Pb Ti0.48 Zr0.52'
_chemical_name_systematic        'Pb (Zr0.52 Ti0.48) O3'
_space_group_IT_number           8
_symmetry_space_group_name_Hall  'C -2y'
_symmetry_space_group_name_H-M   'C 1 m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.493
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.7154
_cell_length_b                   5.704
_cell_length_c                   4.1378
_cell_volume                     134.890
_citation_journal_id_ASTM        APCPCS
_cod_data_source_file            Dmowski_APCPCS_2001_1447.cif
_cod_data_source_block           O3Pb1Ti0.48Zr0.52
_cod_original_cell_volume        134.89
_cod_original_formula_sum        'O3 Pb1 Ti0.48 Zr0.52'
_cod_database_code               1525908
Structural and magnetic properties of Pr Fe12-x Vx and their nitrides
Mao, W.; Zhang, X.; Ji, C.; Cheng, B.; Zhang, B.; Wang, L.; Yang, Y.; Xue, Y.; Du, H.; Li, F.; Acta Materialia 49 (2001) 721–728; doi:10.1016/S1359-6454(00)00354-2

data_1525909
_publ_section_title
;
 Structural and magnetic properties of Pr Fe12-x Vx and their nitrides
;
_journal_issue                   4
_journal_name_full               'Acta Materialia'
_journal_page_first              721
_journal_page_last               728
_journal_paper_doi               10.1016/S1359-6454(00)00354-2
_journal_volume                  49
_journal_year                    2001
_chemical_formula_sum            'Fe10.84 N0.43 Pr V1.16'
_chemical_name_systematic        'Pr Fe10.84 V1.16 N0.43'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.593
_cell_length_b                   8.593
_cell_length_c                   4.812
_cell_volume                     355.316
_citation_journal_id_ASTM        ACMAFD
_cod_data_source_file            Mao_ACMAFD_2001_874.cif
_cod_data_source_block           Fe10.84N0.43Pr1V1.16
_cod_original_cell_volume        355.3164
_cod_original_formula_sum        'Fe10.84 N0.43 Pr1 V1.16'
_cod_database_code               1525909
Structure of Pb (Zr, Ti) O3 near the morphotropic phase boundary
Dmowski, W.; Egami, T.; Farber, L.; Davies, P.K.; AIP Conference Proceedings 582 (2001) 33–44; doi:

data_1525910
_publ_section_title
;
 Structure of Pb (Zr, Ti) O3 near the morphotropic phase boundary
;
_journal_name_full               'AIP Conference Proceedings'
_journal_page_first              33
_journal_page_last               44
_journal_volume                  582
_journal_year                    2001
_chemical_formula_sum            'O3 Pb Ti0.4 Zr0.6'
_chemical_name_systematic        'Pb (Zr0.6 Ti0.4) O3'
_space_group_IT_number           161
_symmetry_space_group_name_Hall  'R 3 -2"c'
_symmetry_space_group_name_H-M   'R 3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   5.756
_cell_length_b                   5.756
_cell_length_c                   14.242
_cell_volume                     408.642
_citation_journal_id_ASTM        APCPCS
_cod_data_source_file            Dmowski_APCPCS_2001_1448.cif
_cod_data_source_block           O3Pb1Ti0.4Zr0.6
_cod_original_cell_volume        408.6422
_cod_original_formula_sum        'O3 Pb1 Ti0.4 Zr0.6'
_cod_database_code               1525910
Synthesis, crystal structure and chemical bonding of a new La - In - Ge ternary phase: La11 In6 Ge4
Mao, J.-G.; Guloy, A.M.; Journal of Alloys Compd. 322 (2001) 135–142; doi:

data_1525911
_publ_section_title
;
 Synthesis, crystal structure and chemical bonding of a new La - In - Ge
 ternary phase: La11 In6 Ge4
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              135
_journal_page_last               142
_journal_volume                  322
_journal_year                    2001
_chemical_formula_sum            'Ge4 In6 La11'
_chemical_name_systematic        'La11 In6 Ge4'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.073
_cell_length_b                   12.073
_cell_length_c                   16.829
_cell_volume                     2452.950
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Mao_JALCEU_2001_1272.cif
_cod_data_source_block           Ge4In6La11
_cod_original_cell_volume        2452.95
_cod_database_code               1525911
Magnetic and neutron diffraction study on ordered perovskites Sr2 Ln Ru O6 (Ln = Tb, Ho)
Doi, Y.; Morii, Y.; Hinatsu, Y.; Oikawa, K.; Shimojo, Y.; Journal of Alloys Compd. 323 (2001) 455–459; doi:

data_1525912
_publ_section_title
;
 Magnetic and neutron diffraction study on ordered perovskites Sr2 Ln Ru
 O6 (Ln = Tb, Ho)
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              455
_journal_page_last               459
_journal_volume                  323
_journal_year                    2001
_chemical_formula_sum            'O6 Ru Sr2 Tb'
_chemical_name_systematic        'Sr2 (Tb Ru O6)'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.249
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.7932
_cell_length_b                   5.8107
_cell_length_c                   8.2011
_cell_volume                     276.067
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Doi_JALCEU_2001_1308.cif
_cod_data_source_block           O6Ru1Sr2Tb1
_cod_original_cell_volume        276.0673
_cod_original_sg_symbol_Hall     '-P 2ybc (x-z,y,z)'
_cod_original_formula_sum        'O6 Ru1 Sr2 Tb1'
_cod_database_code               1525912
Structure cristalline de Na2 Sb4 O7 , etude comparative de l'influe de la paire non liee sur l'environnement de l'atome d'antimoine(III) dans quelques antimoniates(III) alcalins
Maraine, P.; Perez, G.; Acta Crystallographica B (24,1968-38,1982) 33 (1977) 1158–1163; doi:

data_2106189
_publ_section_title
;
 Structure cristalline de Na2 Sb4 O7 , etude comparative de l'influe de la
 paire non liee sur l'environnement de l'atome d'antimoine(III) dans
 quelques antimoniates(III) alcalins
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              1158
_journal_page_last               1163
_journal_volume                  33
_journal_year                    1977
_chemical_formula_sum            'Na2 O7 Sb4'
_chemical_name_systematic        'Na2 (Sb4 O7)'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 149.4
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.03
_cell_length_b                   16.92
_cell_length_c                   9.64
_cell_volume                     915.811
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            Maraine_ACBCAR_1977_88.cif
_cod_data_source_block           Na2O7Sb4
_cod_original_cell_volume        915.8115
_cod_database_code               2106189
Crystal structures and magnetic properties of the 6H-perovskites Ba3 Ln Ru2 O9 (Ln = Ce, Pr and Tb)
Doi, Y.; Wakeshima, M.; Tobo, A.; Hinatsu, Y.; Ohoyama, K.; Yamaguchi, Y.; Journal of Materials Chemistry 11 (2001) 3135–3140; doi:

data_7221279
_publ_section_title
;
 Crystal structures and magnetic properties of the 6H-perovskites Ba3 Ln
 Ru2 O9 (Ln = Ce, Pr and Tb)
;
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              3135
_journal_page_last               3140
_journal_volume                  11
_journal_year                    2001
_chemical_formula_sum            'Ba3 Ce O9 Ru2'
_chemical_name_systematic        'Ba3 Ce Ru2 O9'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   5.8894
_cell_length_b                   5.8894
_cell_length_c                   14.6476
_cell_volume                     439.986
_citation_journal_id_ASTM        JMACEP
_cod_data_source_file            Doi_JMACEP_2001_1803.cif
_cod_data_source_block           Ba3Ce1O9Ru2
_cod_original_cell_volume        439.9864
_cod_original_formula_sum        'Ba3 Ce1 O9 Ru2'
_cod_database_code               7221279